LMucko/crystallography-open-database huggingface dataset:
Muscovite- and phengite-3T: crystal structure and conditions of formation
Amisano-Canesi A; Chiari, G.; Ferraris, G.; Ivaldi, G.; Soboleva, S. V.; European Journal of Mineralogy 6 (1994) 489–496; doi:

data_9005201
_publ_section_title
;
 Muscovite- and phengite-3T: crystal structure and conditions of formation
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              489
_journal_page_last               496
_journal_volume                  6
_journal_year                    1994
_chemical_compound_source        Dora-Maira
_chemical_formula_sum
'Al1.87 H2 K0.92 Mg0.6 Na0.01 O12 Si3.54 Ti0.02'
_chemical_name_mineral           Muscovite-3T
_space_group_IT_number           151
_symmetry_space_group_name_Hall  'P 31 2 (0 0 4)'
_symmetry_space_group_name_H-M   'P 31 1 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   5.212
_cell_length_b                   5.212
_cell_length_c                   29.804
_cell_volume                     701.155
_database_code_amcsd             0006547
_exptl_crystal_density_diffrn    2.811
_cod_original_formula_sum        'K.92 Na.01 Al1.87 Mg.6 Ti.02 Si3.54 O12 H2'
_cod_database_code               9005201
Crystal structure and microtwinning of K-rich nenadkevichite Note: Wat4 y-coordinate changed to reproduce reported bond lengths
Rastsvetaeva, R. K.; Tamazyan, R. A.; Pushcharovsky, D. Y.; Nadezhina, T. N.; European Journal of Mineralogy 6 (1994) 503–509; doi:

data_9005202
_publ_section_title
;
 Crystal structure and microtwinning of K-rich nenadkevichite
 Note: Wat4 y-coordinate changed to reproduce reported bond lengths
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              503
_journal_page_last               509
_journal_volume                  6
_journal_year                    1994
_chemical_formula_sum            'H13.2 K2.98 Na1.22 Nb2.2 O31.15 Si8 Ti1.8'
_chemical_name_mineral           Nenadkevichite
_space_group_IT_number           8
_symmetry_space_group_name_Hall  'C -2y'
_symmetry_space_group_name_H-M   'C 1 m 1'
_cell_angle_alpha                90
_cell_angle_beta                 117.87
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   14.692
_cell_length_b                   14.164
_cell_length_c                   7.859
_cell_volume                     1445.745
_database_code_amcsd             0006548
_exptl_crystal_density_diffrn    2.691
_cod_original_formula_sum        'K2.98 Na1.22 (Nb2.2 Ti1.8) Si8 O31.15 H13.2'
_cod_database_code               9005202
Temperature dependence of the cation distribution in CoAl2O4 spinel Quenched from T = 700 C
O'Neill H St C; European Journal of Mineralogy 6 (1994) 603–609; doi:

data_9005203
_publ_section_title
;
 Temperature dependence of the cation distribution in CoAl2O4 spinel
 Quenched from T = 700 C
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              603
_journal_page_last               609
_journal_volume                  6
_journal_year                    1994
_chemical_formula_sum            'Al2 Co O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.10658
_cell_length_b                   8.10658
_cell_length_c                   8.10658
_cell_volume                     532.737
_database_code_amcsd             0006549
_exptl_crystal_density_diffrn    4.411
_exptl_crystal_thermal_history   'Quenched from T = 700 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Co Al2) O4'
_cod_database_code               9005203
Temperature dependence of the cation distribution in CoAl2O4 spinel Quenched from T = 750 C
O'Neill H St C; European Journal of Mineralogy 6 (1994) 603–609; doi:

data_9005204
_publ_section_title
;
 Temperature dependence of the cation distribution in CoAl2O4 spinel
 Quenched from T = 750 C
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              603
_journal_page_last               609
_journal_volume                  6
_journal_year                    1994
_chemical_formula_sum            'Al2 Co O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.10650
_cell_length_b                   8.10650
_cell_length_c                   8.10650
_cell_volume                     532.721
_database_code_amcsd             0006550
_exptl_crystal_density_diffrn    4.411
_exptl_crystal_thermal_history   'Quenched from T = 750 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Co Al2) O4'
_cod_database_code               9005204
Temperature dependence of the cation distribution in CoAl2O4 spinel Quenched from T = 800 C data set 1
O'Neill H St C; European Journal of Mineralogy 6 (1994) 603–609; doi:

data_9005205
_publ_section_title
;
 Temperature dependence of the cation distribution in CoAl2O4 spinel
 Quenched from T = 800 C  data set 1
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              603
_journal_page_last               609
_journal_volume                  6
_journal_year                    1994
_chemical_formula_sum            'Al2 Co O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.10670
_cell_length_b                   8.10670
_cell_length_c                   8.10670
_cell_volume                     532.761
_database_code_amcsd             0006551
_exptl_crystal_density_diffrn    4.411
_exptl_crystal_thermal_history   'Quenched from T = 800 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Co Al2) O4'
_cod_database_code               9005205
Temperature dependence of the cation distribution in CoAl2O4 spinel Quenched from T = 800 C data set 2
O'Neill H St C; European Journal of Mineralogy 6 (1994) 603–609; doi:

data_9005206
_publ_section_title
;
 Temperature dependence of the cation distribution in CoAl2O4 spinel
 Quenched from T = 800 C  data set 2
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              603
_journal_page_last               609
_journal_volume                  6
_journal_year                    1994
_chemical_formula_sum            'Al2 Co O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.10670
_cell_length_b                   8.10670
_cell_length_c                   8.10670
_cell_volume                     532.761
_database_code_amcsd             0006552
_exptl_crystal_density_diffrn    4.411
_exptl_crystal_thermal_history   'Quenched from T = 800 C'
_cod_duplicate_entry             9005205
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Co Al2) O4'
_cod_database_code               9005206
Temperature dependence of the cation distribution in CoAl2O4 spinel Quenched from T = 850 C
O'Neill H St C; European Journal of Mineralogy 6 (1994) 603–609; doi:

data_9005207
_publ_section_title
;
 Temperature dependence of the cation distribution in CoAl2O4 spinel
 Quenched from T = 850 C
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              603
_journal_page_last               609
_journal_volume                  6
_journal_year                    1994
_chemical_formula_sum            'Al2 Co O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.10664
_cell_length_b                   8.10664
_cell_length_c                   8.10664
_cell_volume                     532.749
_database_code_amcsd             0006553
_exptl_crystal_density_diffrn    4.411
_exptl_crystal_thermal_history   'Quenched from T = 850 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Co Al2) O4'
_cod_database_code               9005207
Temperature dependence of the cation distribution in CoAl2O4 spinel Quenched from T = 900 C data set 1
O'Neill H St C; European Journal of Mineralogy 6 (1994) 603–609; doi:

data_9005208
_publ_section_title
;
 Temperature dependence of the cation distribution in CoAl2O4 spinel
 Quenched from T = 900 C  data set 1
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              603
_journal_page_last               609
_journal_volume                  6
_journal_year                    1994
_chemical_formula_sum            'Al2 Co O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.10664
_cell_length_b                   8.10664
_cell_length_c                   8.10664
_cell_volume                     532.749
_database_code_amcsd             0006554
_exptl_crystal_density_diffrn    4.411
_exptl_crystal_thermal_history   'Quenched from T = 900 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Co Al2) O4'
_cod_database_code               9005208
Temperature dependence of the cation distribution in CoAl2O4 spinel Quenched from T = 900 C data set 2
O'Neill H St C; European Journal of Mineralogy 6 (1994) 603–609; doi:

data_9005209
_publ_section_title
;
 Temperature dependence of the cation distribution in CoAl2O4 spinel
 Quenched from T = 900 C  data set 2
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              603
_journal_page_last               609
_journal_volume                  6
_journal_year                    1994
_chemical_formula_sum            'Al2 Co O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.10664
_cell_length_b                   8.10664
_cell_length_c                   8.10664
_cell_volume                     532.749
_database_code_amcsd             0006555
_exptl_crystal_density_diffrn    4.411
_exptl_crystal_thermal_history   'Quenched from T = 900 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Co Al2) O4'
_cod_database_code               9005209
Temperature dependence of the cation distribution in CoAl2O4 spinel Quenched from T = 900 C data set 3
O'Neill H St C; European Journal of Mineralogy 6 (1994) 603–609; doi:

data_9005210
_publ_section_title
;
 Temperature dependence of the cation distribution in CoAl2O4 spinel
 Quenched from T = 900 C  data set 3
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              603
_journal_page_last               609
_journal_volume                  6
_journal_year                    1994
_chemical_formula_sum            'Al2 Co O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.10664
_cell_length_b                   8.10664
_cell_length_c                   8.10664
_cell_volume                     532.749
_database_code_amcsd             0006556
_exptl_crystal_density_diffrn    4.411
_exptl_crystal_thermal_history   'Quenched from T = 900 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Co Al2) O4'
_cod_database_code               9005210
Temperature dependence of the cation distribution in CoAl2O4 spinel Quenched from T = 950 C
O'Neill H St C; European Journal of Mineralogy 6 (1994) 603–609; doi:

data_9005211
_publ_section_title
;
 Temperature dependence of the cation distribution in CoAl2O4 spinel
 Quenched from T = 950 C
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              603
_journal_page_last               609
_journal_volume                  6
_journal_year                    1994
_chemical_formula_sum            'Al2 Co O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.10688
_cell_length_b                   8.10688
_cell_length_c                   8.10688
_cell_volume                     532.796
_database_code_amcsd             0006557
_exptl_crystal_density_diffrn    4.411
_exptl_crystal_thermal_history   'Quenched from T = 950 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Co Al2) O4'
_cod_database_code               9005211
Temperature dependence of the cation distribution in CoAl2O4 spinel Quenched from T = 1000 C
O'Neill H St C; European Journal of Mineralogy 6 (1994) 603–609; doi:

data_9005212
_publ_section_title
;
 Temperature dependence of the cation distribution in CoAl2O4 spinel
 Quenched from T = 1000 C
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              603
_journal_page_last               609
_journal_volume                  6
_journal_year                    1994
_chemical_formula_sum            'Al2 Co O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.10630
_cell_length_b                   8.10630
_cell_length_c                   8.10630
_cell_volume                     532.682
_database_code_amcsd             0006558
_exptl_crystal_density_diffrn    4.411
_exptl_crystal_thermal_history   'Quenched from T = 1000 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Co Al2) O4'
_cod_database_code               9005212
_amcsd_formula_title             CoAl2O4
Temperature dependence of the cation distribution in CoAl2O4 spinel Quenched from T = 1050 C data set 1
O'Neill H St C; European Journal of Mineralogy 6 (1994) 603–609; doi:

data_9005213
_publ_section_title
;
 Temperature dependence of the cation distribution in CoAl2O4 spinel
 Quenched from T = 1050 C  data set 1
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              603
_journal_page_last               609
_journal_volume                  6
_journal_year                    1994
_chemical_formula_sum            'Al2 Co O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.10669
_cell_length_b                   8.10669
_cell_length_c                   8.10669
_cell_volume                     532.759
_database_code_amcsd             0006559
_exptl_crystal_density_diffrn    4.411
_exptl_crystal_thermal_history   'Quenched from T = 1050 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Co Al2) O4'
_cod_database_code               9005213
Temperature dependence of the cation distribution in CoAl2O4 spinel Quenched from T = 1050 C data set 2
O'Neill H St C; European Journal of Mineralogy 6 (1994) 603–609; doi:

data_9005214
_publ_section_title
;
 Temperature dependence of the cation distribution in CoAl2O4 spinel
 Quenched from T = 1050 C  data set 2
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              603
_journal_page_last               609
_journal_volume                  6
_journal_year                    1994
_chemical_formula_sum            'Al2 Co O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.10669
_cell_length_b                   8.10669
_cell_length_c                   8.10669
_cell_volume                     532.759
_database_code_amcsd             0006560
_exptl_crystal_density_diffrn    4.411
_exptl_crystal_thermal_history   'Quenched from T = 1050 C'
_cod_duplicate_entry             9005213
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Co Al2) O4'
_cod_database_code               9005214
Temperature dependence of the cation distribution in CoAl2O4 spinel Quenched from T = 1050 C data set 3
O'Neill H St C; European Journal of Mineralogy 6 (1994) 603–609; doi:

data_9005215
_publ_section_title
;
 Temperature dependence of the cation distribution in CoAl2O4 spinel
 Quenched from T = 1050 C  data set 3
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              603
_journal_page_last               609
_journal_volume                  6
_journal_year                    1994
_chemical_formula_sum            'Al2 Co O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.10669
_cell_length_b                   8.10669
_cell_length_c                   8.10669
_cell_volume                     532.759
_database_code_amcsd             0006561
_exptl_crystal_density_diffrn    4.411
_exptl_crystal_thermal_history   'Quenched from T = 1050 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Co Al2) O4'
_cod_database_code               9005215
Temperature dependence of the cation distribution in CoAl2O4 spinel Quenched from T = 1100 C
O'Neill H St C; European Journal of Mineralogy 6 (1994) 603–609; doi:

data_9005216
_publ_section_title
;
 Temperature dependence of the cation distribution in CoAl2O4 spinel
 Quenched from T = 1100 C
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              603
_journal_page_last               609
_journal_volume                  6
_journal_year                    1994
_chemical_formula_sum            'Al2 Co O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.10673
_cell_length_b                   8.10673
_cell_length_c                   8.10673
_cell_volume                     532.767
_database_code_amcsd             0006562
_exptl_crystal_density_diffrn    4.411
_exptl_crystal_thermal_history   'Quenched from T = 1100 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Co Al2) O4'
_cod_database_code               9005216
Temperature dependence of the cation distribution in CoAl2O4 spinel Quenched from T = 1150 C data set 1
O'Neill H St C; European Journal of Mineralogy 6 (1994) 603–609; doi:

data_9005217
_publ_section_title
;
 Temperature dependence of the cation distribution in CoAl2O4 spinel
 Quenched from T = 1150 C data set 1
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              603
_journal_page_last               609
_journal_volume                  6
_journal_year                    1994
_chemical_formula_sum            'Al2 Co O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.10683
_cell_length_b                   8.10683
_cell_length_c                   8.10683
_cell_volume                     532.786
_database_code_amcsd             0006563
_exptl_crystal_density_diffrn    4.411
_exptl_crystal_thermal_history   'Quenched from T = 1150 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Co Al2) O4'
_cod_database_code               9005217
Temperature dependence of the cation distribution in CoAl2O4 spinel Quenched from T = 1150 C data set 2
O'Neill H St C; European Journal of Mineralogy 6 (1994) 603–609; doi:

data_9005218
_publ_section_title
;
 Temperature dependence of the cation distribution in CoAl2O4 spinel
 Quenched from T = 1150 C data set 2
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              603
_journal_page_last               609
_journal_volume                  6
_journal_year                    1994
_chemical_formula_sum            'Al2 Co O4'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.10683
_cell_length_b                   8.10683
_cell_length_c                   8.10683
_cell_volume                     532.786
_database_code_amcsd             0006564
_exptl_crystal_density_diffrn    4.411
_exptl_crystal_thermal_history   'Quenched from T = 1150 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Co Al2) O4'
_cod_database_code               9005218